- About this Journal ·
- Abstracting and Indexing ·
- Aims and Scope ·
- Annual Issues ·
- Article Processing Charges ·
- Articles in Press ·
- Author Guidelines ·
- Bibliographic Information ·
- Citations to this Journal ·
- Contact Information ·
- Editorial Board ·
- Editorial Workflow ·
- Free eTOC Alerts ·
- Publication Ethics ·
- Reviewers Acknowledgment ·
- Submit a Manuscript ·
- Subscription Information ·
- Table of Contents
Journal of Nanomaterials
Volume 2014 (2014), Article ID 307687, 6 pages
Annealing Effects on Photocatalytic Activity of Zn0.2Cd0.8S Films Prepared by Chemical Bath Deposition
Department of Applied Physics, Key Laboratory for Micro-Nano Physics and Technology of Hunan Province, Hunan University, Changsha 410082, China
Received 14 April 2014; Accepted 18 June 2014; Published 3 July 2014
Academic Editor: Anukorn Phuruangrat
Copyright © 2014 Yi-Feng Chai et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
Zn0.2Cd0.8S alloyed films were prepared on glass substrates at room temperature using chemical bath deposition method. The obtained films were annealed at temperatures ranging from 200°C to 500°C with heating rate of 5°C/min and annealed at 400°C with heating rate of 2°C/min and 10°C/min. The films were characterized by X-ray diffraction, scanning electron microscopy, energy-dispersive spectroscopy, and UV-VIS spectrophotometer. The increasing of annealing temperature increases the crystallinity and the mean grain size of Zn0.2Cd0.8S alloyed films and significantly enhances the absorption in the visible region. The efficient visible light photocatalytic activity for annealed Zn0.2Cd0.8S alloyed films is associated with the larger size grain and the higher crystallinity.
Semiconductor assisted photocatalysis has received increasing attention owing to its potential in simultaneously solving the energy shortage and environmental problems [1–3]. Among the various semiconductors for photocatalysis, TiO2 is undoubtedly the most widely used photocatalyst. However, the wide band gap and rapid electron-hole recombination of TiO2 largely limits its application as a photocatalyst [4–6]. In order to utilize the abundant solar energy, the development of visible light active photocatalysts with high activities under visible light irradiation is of great importance. To date, many semiconductor photocatalyst systems have been reported to be active under visible light, such as modified TiO2 and its composites [7, 8], CdS [9, 10], ZnS [11, 12], SrSnO3 , Bi2WO6 , SrTiO3 , , , AgInS2 , Ag3PO4 , and ZuS–CuInS2–AgInS2 . Among them, solid solution photocatalyst has been extensively studied due to its controllable band structure and excellent performance in the photocatalytic hydrogen production process under visible light irradiation [21, 22]. In our previous work, it is found that the alloyed films show enhanced photocatalytic activity when = 0.20~0.29 [23, 24].
Heat treatment is often used to tune the structure and properties of materials. By using appropriate parameters for heat treatment, different shapes  or colors  of nanomaterials with controllable properties can be produced. However, the systematic effects of annealing on the structural and photocatalytic properties of alloyed films were rarely reported. In order to clarify this issue, Zn0.2Cd0.8S alloyed films are synthesized by a simple chemical bath deposition and the effects of annealing temperature and heating rate on the morphology, composition, and optical properties are comprehensively explored in this work. It is interesting that shape and particle size can be controlled by annealing temperature and heating rate which greatly influences the photocatalytic activity of Zn0.2Cd0.8S alloyed films. The photocatalytic activity of Zn0.2Cd0.8S alloyed films under visible light irradiation is greatly enhanced by increase of annealing temperature and heating rate.
2.1. Preparations of Zn0.2Cd0.8S Thin Films
All the chemicals are analytical reagents and used without further purification. The glass slides were cleaned with acetone, alcohol, and deionized water, respectively. 0.005 M ZnSO4 · 7H2O and 0.02 M CdCl2 were mixed in a beaker together with appropriate amount of SC(NH2)2 and NH4Cl. The pH of the aqueous solution was adjusted to about 12 with ammonia water. A clear and homogeneous solution was obtained after stirring for several minutes. Then, the glass slides were put into the above solution and the deposition was kept at 80°C for 3 h. Finally, the synthesized films were dried in vacuum at 60°C for 1 h. The nominal molar ratios of Zn/Cd were 1/4, and the prepared films were marked as Zn0.2Cd0.8S. The as-prepared Zn0.2Cd0.8S films were annealed at different temperatures and heating rates for 1 h in the 98% Ar + 2% H2 atmosphere.
The structure was characterized by X-ray diffraction (XRD, D8). The morphologies of the products were characterized by scanning electron microscopy (SEM, Hitachi S-4800) and the components were measured by energy-dispersive spectroscopy (EDS). The fluorescence (FL) spectra were obtained by fluorescence spectrophotometer (F-2500) with an excitation wavelength of 380 nm laser line. The absorption spectra of the films were determined using a double beam UV-VIS spectrophotometer (TU-1901) in the wavelength range of 300–800 nm.
2.3. Photodegradation Tests
The photocatalytic activity of Zn0.2Cd0.8S films was evaluated by photodegradation of aqueous solution of methyl orange under the irradiation of 55 W LED lamps. The catalytic experiments were carried out with 60 ML methyl orange solution and annealed Zn0.2Cd0.8S films. The suspension was magnetically stirred and placed at 3 cm from the lamp. During irradiation, the samples were withdrawn at regular time intervals and centrifuged to remove the catalysts. The absorption spectra of the solution were determined using UV-VIS spectrophotometer.
3. Results and Discussions
3.1. Crystal Structure and Morphology
SEM images of Zn0.2Cd0.8S alloyed films at different annealing conditions are delineated in Figure 1. As can be seen in Figures 1(a) and 1(b), as the annealing temperature is lower than 300°C, Zn0.2Cd0.8S alloyed films are dense, uniform, and homogeneous without detectable pores and covered well with glass substrate. However, the grains become bigger and cracks appear with increasing the annealing temperature or the heating rate as shown in Figures 1(c), 1(d), and 1(c2), which may be due to the increasing stress with the increasing temperature, which is similar to that reported for ZnS .
Zn0.2Cd0.8S alloyed films were characterized by XRD to obtain information about the structure of the products. Figure 2 shows that the XRD patterns can be indexed as hexagonal structures (JCPDS No.49–1302) with the five characteristic diffraction peaks matching with the (100), (002), (101), (110), and (112) crystalline plane of CdS. The strong diffraction peaks indicate that all samples showed good crystalline structure and large mean grain size. With increasing the annealing temperature and heating rate, the CdS diffraction peaks become more distinct and the full width at half maximum narrows. This implies the increase of the crystallinity and the mean grain size of Zn0.2Cd0.8S.
3.2. Optical Properties
The optical absorption spectra of Zn0.2Cd0.8S alloyed films annealed at different temperatures with different heating rates are illustrated in Figure 3. The absorption edge of Zn0.2Cd0.8S alloyed films is about 520 nm and obviously shifts to longer wavelength, with increasing the annealing temperature and heating rate, which greatly enhance the absorption of Zn0.2Cd0.8S alloyed films in the visible region.
The degradation efficiency is shown in Figure 4. The plot inserted in Figure 4(a) illustrates the typical irradiation time dependent UV-vis spectra of methyl orange solution during photocatalytic degradation. The spectra of methyl orange exhibit a main band with a maximum at 464 nm in the visible region. The absorption peaks of methyl orange gradually decrease with irradiation time during the photocatalytic reaction, indicating the degradation of methyl orange. Therefore, the decrease of absorbance corresponding to the decrease of methyl orange concentration is recorded. The degradation efficiency is calculated according the following equation: Here is the initial concentration of methyl orange (10 mg/L) and is the concentration of methyl orange after an irradiation time. It can be clearly seen from Figure 4(a) that the degradation efficiency increases continuously with irradiation time. The degradation efficiency of methyl orange for Zn0.2Cd0.8S films is 18.50%, 51.08%, 57.01%, and 63.75%, respectively, for the samples annealed at 200°C, 300°C, 400°C, and 500°C after 4 h visible light irradiation. The degradation efficiency of methyl orange for Zn0.2Cd0.8S alloyed films is 32.64%, 57.01%, 65.78%, respectively, for the samples annealed at 400°C with heating rate of 2°C/min, 5°C/min, and 10 °C/min (Figure 4(b)) after 4 h visible light irradiation. It is obvious that the degradation efficiency increases with an increase of heating rate. These results suggest that the photocatalytic activity of Zn0.2Cd0.8S alloyed films can be extremely improved by appropriate annealing conditions.
It is known that the photoactivity of semiconductors is particle size-dependent [27, 28] and crystallinity-dependent [29, 30]. The grain size increases in Figure 1 and the peak intensity of XRD patterns in Figure 2 increases with the increasing temperature and heating rate, suggesting the larger grain size and the higher crystallinity. Thus, the higher photoactivity can be attributed to the larger size and the higher crystallinity of annealed Zn0.2Cd0.8S alloyed films, which decreases electron-hole recombination centers, facilitates the separation of electron-hole pairs, and therefore enhances the photoactivity of Zn0.2Cd0.8S alloyed films.
Zn0.2Cd0.8S alloyed films prepared by simple chemical bath deposition method were studied as photocatalysts for degradation of methyl orange under visible light irradiation. The grain size increases and crystallinity is enhanced for the Zn0.2Cd0.8S alloyed films with increasing annealing temperature and heating rate. Moreover the absorption edge obviously shifts to longer wavelength with increasing the annealing temperature and the heating rate. Increasing the annealing temperature and the heating rate can enhance photocatalytic activities of Zn0.2Cd0.8S alloyed films under visible light irradiation. This work provides a simple and efficient method to enhance the photocatalytic activity of semiconductors.
Conflict of Interests
The authors declare that there is no conflict of interests regarding the publication of this paper.
This work was supported by the National Natural Science Foundation of China (Grant nos. 11074069, 61176116), the Hunan Provincial Natural Science Foundation of China (Grant no. 12JJ3009), and Aid program for Science and Technology Innovative Research Team in Higher Educational Institutions of Hunan Province.
- X. J. Liu, L. K. Pan, T. Lv, and Z. Sun, “CdS sensitized TiO2 film for photocatalytic reduction of Cr(VI) by microwave-assisted chemical bath deposition method,” Journal of Alloys and Compounds, vol. 583, pp. 390–395, 2014.
- X. Chen, S. Shen, L. Guo, and S. S. Mao, “Semiconductor-based photocatalytic hydrogen generation,” Chemical Reviews, vol. 110, no. 11, pp. 6503–6570, 2010.
- J. G. Yu, M. Jaroniec, H. G. Yu, and W. H. Fan, “Synthesis, characterization, properties, and applications of nanosized photocatalytic materials,” Journal of Nanomaterials, vol. 2012, Article ID 783686, 3 pages, 2012.
- H. Tong, S. Ouyang, Y. Bi, N. Umezawa, M. Oshikiri, and J. Ye, “Nano-photocatalytic materials: Possibilities and challenges,” Advanced Materials, vol. 24, no. 2, pp. 229–251, 2012.
- S. A. Elfeky and A. S. A. Al-Sherbini, “Photo-oxidation of rhodamine-6-G via TiO2 and Au/TiO2-bound polythene beads,” Journal of Nanomaterials, vol. 2011, Article ID 570438, 8 pages, 2011.
- Y. Chen, G. Huang, W. Huang, B. S. Zou, and A. Pan, “Enhanced visible-light photoactivity of La-doped ZnS thin films,” Applied Physics A: Materials Science and Processing, vol. 108, no. 4, pp. 895–900, 2012.
- Z. Zhang, L. Zhang, M. N. Hedhili, H. Zhang, and P. Wang, “Plasmonic gold nanocrystals coupled with photonic crystal seamlessly on TiO2 nanotube photoelectrodes for efficient visible light photoelectrochemical water splitting,” Nano Letters, vol. 13, no. 1, pp. 14–20, 2013.
- H. B. Wu, H. H. Hng, and X. W. D. Lou, “Direct synthesis of anatase TiO2 nanowires with enhanced photocatalytic activity,” Advanced Materials, vol. 24, no. 19, pp. 2567–2571, 2012.
- N. Bao, L. Shen, T. Takata, and K. Domen, “Self-templated synthesis of nanoporous CdS nanostructures for highly efficient photocatalytic hydrogen production under visible light,” Chemistry of Materials, vol. 20, no. 1, pp. 110–117, 2008.
- S. H. Mohamed and E. R. Shaaban, “Microstructural, optical and photocatalytic properties of CdS doped TiO2 thin films,” Physica B: Condensed Matter, vol. 406, no. 22, pp. 4327–4331, 2011.
- Y. Chen, G. F. Huang, W. Q. Huang et al., “Annealing effects on photocatalytic activity of ZnS films prepared by chemical bath deposition,” Materials Letters, vol. 75, pp. 221–224, 2012.
- J. Zhang, J. Yu, Y. Zhang, Q. Li, and J. R. Gong, “Visible light photocatalytic H2-production activity of CuS/ZnS porous nanosheets based on photoinduced interfacial charge transfer,” Nano Letters, vol. 11, no. 11, pp. 4774–4779, 2011.
- D. Chen and J. Ye, “SrSnO3 nanostructures: synthesis, characterization, and photocatalytic properties,” Chemistry of Materials, vol. 19, no. 18, pp. 4585–4591, 2007.
- S. Sun, W. Wang, and L. Zhang, “Facile preparation of three-dimensionally ordered macroporous Bi2WO6 with high photocatalytic activity,” Journal of Materials Chemistry, vol. 22, no. 36, pp. 19244–19249, 2012.
- S. T. Christensen, J. W. Elam, B. Lee, Z. Feng, M. J. Bedzyk, and M. C. Hersam, “Nanoscale structure and morphology of atomic layer deposition platinum on SrTiO3 (001),” Chemistry of Materials, vol. 21, no. 3, pp. 516–521, 2009.
- J. Pan, M. I. B. Utama, Q. Zhang et al., “Composition-tunable vertically aligned CdSxSe1−x nanowire arrays via van der Waals epitaxy: Investigation of optical properties and photocatalytic behavior,” Advanced Materials, vol. 24, no. 30, pp. 4151–4156, 2012.
- J. Zhang, J. Yu, M. Jaroniec, and J. R. Gong, “Noble metal-free reduced graphene oxide-ZnxCd1-xS nanocomposite with enhanced solar photocatalytic H2-production performance,” Nano Letters, vol. 12, no. 9, pp. 4584–4589, 2012.
- T. Torimoto, T. Kameyama, and S. Kuwabata, “Photofunctional materials fabricated with chalcopyrite-type semiconductor nanoparticles composed of AgInS2 and its solid solutions,” Journal of Physical Chemistry Letters, vol. 5, no. 2, pp. 336–347, 2014.
- G. F. Huang, Z. L. Ma, W. Q. Huang et al., “Ag3PO4 semiconductor photocatalyst: possibilities and challenges,” Journal of Nanomaterials, vol. 2013, Article ID 371356, 8 pages, 2013.
- I. Tsuji, H. Kato, and A. Kudo, “Photocatalytic hydrogen evolution on ZnS-CuInS2-AglnS2 solid solution photocatalysts with wide visible light absorption bands,” Chemistry of Materials, vol. 18, no. 7, pp. 1969–1975, 2006.
- L. Wang, W. Wang, M. Shang, W. Yin, S. Sun, and L. Zhang, “Enhanced photocatalytic hydrogen evolution under visible light over Cd1-xZnxS solid solution with cubic zinc blend phase,” International Journal of Hydrogen Energy, vol. 35, no. 1, pp. 19–25, 2010.
- W. Li, D. Li, W. Zhang, Y. Hu, Y. He, and X. Fu, “Microwave synthesis of ZnxCd1-xS nanorods and their photocatalytic activity under visible light,” Journal of Physical Chemistry C, vol. 114, no. 5, pp. 2154–2159, 2010.
- K. Zhang, D. Jing, C. Xing, and L. Guo, “Significantly improved photocatalytic hydrogen production activity over Cd1 - xZnxS photocatalysts prepared by a novel thermal sulfuration method,” International Journal of Hydrogen Energy, vol. 32, no. 18, pp. 4685–4691, 2007.
- W. Li, D. Li, J. Xian et al., “Specific analyses of the active species on Zn0.28Cd0.72S and TiO2 photocatalysts in the degradation of methyl orange,” Journal of Physical Chemistry C, vol. 114, no. 49, pp. 21482–21492, 2010.
- P. Yang, S. Q. Wang, M. Ando, and N. Murase, “CdSe/Cd1-x ZnxS core/shell quantum dots with tunable emission: growth and morphology evolution,” Journal of Materials Science, vol. 48, no. 2, pp. 651–658, 2013.
- R. Sethi, L. Kumar, P. K. Sharma, and A. C. Pandey, “Tunable visible emission of Ag-doped CdZnS alloy quantum dots,” Nanoscale Research Letters, vol. 5, no. 1, pp. 96–102, 2010.
- A. Datta, A. Priyam, S. N. Bhattacharyya, K. K. Mukherjea, and A. Saha, “Temperature tunability of size in CdS nanoparticles and size dependent photocatalytic degradation of nitroaromatics,” Journal of Colloid and Interface Science, vol. 322, no. 1, pp. 128–135, 2008.
- Y. Tian, G. Huang, L. Tang, M. Xia, W. Huang, and Z. Ma, “Size-controllable synthesis and enhanced photocatalytic activity of porous ZnS nanospheres,” Materials Letters, vol. 83, pp. 104–107, 2012.
- S. Tian, H. Yang, M. Cui et al., “Monodisperse rutile TiO2 nanorod-based microspheres with various diameters: hydrothermal synthesis, formation mechanism and diameter- and crystallinity-dependent photocatalytic properties,” Applied Physics A: Materials Science and Processing, vol. 104, no. 1, pp. 149–158, 2011.
- S. Abdul Rashid, S. H. Othman, T. I. Mohd Ghazi, and N. Abdullah, “Effect of postdeposition heat treatment on the crystallinity, size, and photocatalytic activity of TiO2 nanoparticles produced via chemical vapour deposition,” Journal of Nanomaterials, vol. 2010, Article ID 512785, 10 pages, 2010.